more strict energy conserving scattering processes. Indeed, this interpretation is in agree-ment with the more strict resonance condition in the two-time calculation in comparison to the one-time kinetics, cf. Fig. 5.14 and the s-shell population in Fig. 5.15b.
5.4 Theory-experiment comparison for the
(a) PL and DTS spectra (b) rise times
Fig. 5.18: DTS and PL spectra of an ensemble of InGaAs QDs at a temperature of 10 K (left panel) as well as the corresponding excitation density dependent rise time for vari-ous temperatures (right panel). Pictures courtesy of H. Kurtze and Prof. Dr. M. Bayer, University Dortmund.
to the action of the pump pulse, IDTS = T−TT00. Even though the DTS does not directly map the carrier distribution but is also inﬂuenced by coherent polarization effects, it serves as a good indicator, especially for later times when coherent polarizations are dephased.
An introduction into the theoretical description of pump-probe experiments is given in for example in Ref. [34, 96]. Around the spectral position of the QD resonances an enhanced transmission due to pump pulse action is seen. For all QD resonances a fast rise time is observed, indicating fast carrier relaxation from the GaAs barrier into the QD states. The intermediate time regime (< 2 ns) shows a complicated time dependent dynamics. Here, the population QD states leads to Coulomb renormalizations, mainly resulting in an blue shift of the resonances due to charging of the QDs described by the Hartree interaction (cf.
Chap. 4.1). For later times (> 2ns), exceeding the recombination time of about 1 ns, the carrier distribution seems to be frozen and an enhanced transmission even in higher QD shells is observed.
Temperature and excitation density dependent measurements provide additional informa-tion about the carrier-density regime in the experiment. In Fig. 5.18b the rise time of the ground-state DTS signal, obtained from a mono-exponential ﬁt, is presented. For low
tem-peratures the strong dependence of the rise-time on the excitation density indicates the im-portance of Coulomb scattering processes. The elevated temperature regime above 180 K dominated by phonon scattering processes as it shows almost no density dependence.
In previous discussions about the phonon-bottleneck problem, Urayama et al. [40, 41] con-sidered the Coulomb scattering mechanism for the interpretation of their low-temperature pump-probe measurements. Their conclusion was that due to Auger processes rapid car-rier relaxation in QDs occurs only if electron and hole are captured into the same dot. This process has been named “geminate capture” in these references. In the opposite case of
“non-geminate capture” where electron and hole are captured into different dots, the obser-vation of a phonon bottleneck was explained due to the lack of scattering partners. How-ever, the discussion for QDs did not include the presence of WL states. Even though the DTS data shown in Fig. 5.18 seem to support their ﬁndings for low temperatures, their ar-gument contradicts with the observation of fast rise times for elevated temperatures, which are almost independent of the excitation density (cf. Fig. 5.18b). Thus, to understand the experimental observations including both temperature regimes, two major questions are addressed in the following:
(i) What is the relative importance of carrier-carrier and carrier-phonon scattering pro-cesses in the low carrier-density regime?
(ii) Can the long-lasting features in the DTS spectra be attributed to long-lived popula-tions of QD states?
(i) Efﬁciency of different scattering processes
Even in the low carrier density regime a variety of scattering processes due to carrier-phonon and Coulomb interaction is expected to contribute. However, a comparison of the carrier-phonon interaction with the electron-electron and electron-hole scattering chan-nels provided by the Coulomb interaction is still missing. Being interested in the relative strength of the various relaxation channels, we present a case study considering different carrier distributions that mimic snapshots of the temporal evolution of the populations after the pulse excitation and allows us to compare the corresponding scattering rates.
For the following investigations we consider an ensemble of InGaAs QDs, randomly dis-tributed on the WL plane, each containing two conﬁned shells for electrons as well as for holes. We refer to the ground state as s-shell and to the two-fold degenerate excited state as p-shell. The level spacings are chosen to be 40 meV and 15 meV for electrons and holes, respectively. Furthermore a temperature of 10K and a QD density of 1010/cm2 is consid-ered. In the weak polar coupling InGaAs material (α = 0.06) the LO-phonon energy is 36 meV.
The calculation of the temporal evolution of a carrier distribution, excited by an opti-cal pulse, and including both carrier-carrier and carrier-phonon scattering on a
quantum-kinetic basis, as discussed in Chap. 5.2.2, is not feasible due to numerical complexity.
Instead an estimate for the relative importance of different processes is obtained by consid-ering scattconsid-ering rates for various carrier distributions. To be able to uniquely deﬁne in- and out-scattering rates, we employ the Markov approximation so that the kinetic equation for the carrier populations can be written in terms of scattering rates as
dtfα(t) = (1−fα(t))Sαin(t)−fα(t)Sαout(t). (5.40) Here,αdenotes some state of the QD-WL system being either a QD stateν or a WL state k. For this chapter our focus is on the relaxation of carriers towards the ground state, and therefore we are interested in the in-scattering rate of the s-shell for electrons.
First, a brief review of our treatment of the Coulomb and the carrier-LO-phonon interaction is given. For the Coulomb interaction the in-scattering rate for electrons in second-order Born approximation (SBA, cf. Chap. 4.1) is given by
Sαe,in = 2π
Wαβγδ 2Wαβγδ∗ −δe,λWαβδγ∗
, (5.41) whereλ speciﬁes the band index and β, γ, δ run over all states in a given band (QD and WL states).fαλdescribes the population of a stateαin the bandλ, andλαits single-particle energy. The scattering rates contain direct and exchange contributions as well as Pauli blocking of the initial and ﬁnal states. For the Coulomb matrix elements Wαβγδ a static screening provided by the Lindhard formula is used. Details on the treatment of Coulomb scattering are given in [91, 156]. In the scattering rate (5.41) electron-electron scattering (λ =e) as well as electron-holes scattering (λ = h) is included. One of the goals in this section of this work is a comparison of the relative strength of these processes.
The scattering rates for the carrier-LO-phonon interaction are evaluated in the random phase approximation (RPA) where the phonons are treated as a bath in thermal equilibrium held at a given temperature,
Sαe,in = 2Re
Mαβ fβ t
× NLOe−iωLOτ+ (1 +NLO)eiωLOτ
. (5.42) Here, Mαβ denotes the carrier-LO-phonon interaction matrix elements, ωLO the phonon energy, andNLO the phonon population. For QDs it was shown in Chap. 5.2.1 that it is essential to include polaron effects, i.e. renormalizations of the single particle properties due to the carrier-phonon interaction, which enter the theory as retarded GFsGe,αR(τ).
The interaction matrix elements for the Coulomb interaction, Wαβγδ, as well as for the carrier-LO-phonon interaction,Mαβ, are determined using the envelope function approxi-mation. For details on the wavefunction model used, we refer to Chap. A.1.
( a ) ( b ) ( c ) ( d ) ( e )
Fig. 5.19: Scattering processes contributing the relaxation of an distribution where initially only the p-shell is ﬁlled (a)-(c) and intermediate situations where also the s-shell and WL states are populated (d)-(e).
After optical excitation of the p-shell, the time evolution of the populations towards a steady state distribution is governed by several scattering processes that are schematically shown in Fig. 5.19. For the initial situation, where only the p-shell is populated, the follow-ing processes contribute: Relaxation of an electron into the QD ground state assisted by the scattering of a electron from the QD into delocalized WL states (Fig. 5.19a), the same mechanism assisted by a hole (Fig. 5.19b), and the relaxation by means of LO-phonon emission (Fig. 5.19c). For later stages of the kinetics more processes come into play, like relaxation assisted by a hole in the QD s-shell (Fig. 5.19d) and other scattering processes that lead to a net relaxation of electrons (Fig. 5.19e).
In Fig. 5.20 the in-scattering rates for the electron s-shell are presented as a function of the carrier density excited by the optical pulse. The scattering rates due to Coulomb interaction have been calculated by Michael Lorke. The different cases considered correspond to stages of the temporal evolution of the carrier distribution after optical excitation. Whereas the fully populated p-shell mimics the initial excitation (Fig. 5.20a), scattering processes result in weakly populated s-shell and WL states (Fig. 5.20b). For long times after the pulse most carriers are expected to be in the ground state (Fig. 5.20c).
As expected, we ﬁnd that for very low carrier densities the carrier-phonon scattering dom-inates. With increasing carrier density the electron-hole scattering becomes the most rele-vant relaxation mechanism, independent of the carrier distribution. For the situation under
0 0.2 0.4 0.6 0.8 1 1.2
carrier-phonon electron-electron electron-hole
0 0.2 0.4 0.6 0.8 1 1.2
(c) 0 0.1 0.2 0.3 0.4 0.5 0.6
in-scattering rate Sin for electron s-shell in 1/ps
(c) 0 0.1 0.2 0.3 0.4 0.5 0.6
in-scattering rate Sin for electron s-shell in 1/ps
0 0.05 0.1 0.15 0.2 0.25 0.3 0.35
0 2e+09 4e+09 6e+09 8e+09 1e+10
carrier density in 1/cm2 (a)
0 0.05 0.1 0.15 0.2 0.25 0.3 0.35
0 2e+09 4e+09 6e+09 8e+09 1e+10
carrier density in 1/cm2 (a)
Fig. 5.20: Total in-scattering rate into the s-shell for electrons, considering a carrier distri-bution where only the p-shell is ﬁlled (a), 60% of the carrier density is in the p-shell, 30%
in the s-shell, 10% in the WL (b) and 60% in the s-shell, 30% in the p-shell and 10% in the WL (c).
investigation, all scattering rates decrease when the populations evolve towards a steady state distribution. However, the relative strength of electron-electron and carrier-phonon scattering rates increase at later stages of the temporal evolution. While in the early stage of the evolution carrier-phonon scattering is more efﬁcient than electron-electron scatter-ing, both contributions are comparable for later stages.
For an ensemble of self-assembled QDs under resonant excitation of the p-shell, electron-hole pairs are always excited within the same QD. On the contrary, when electron-electron-hole pairs are excited in the WL, electrons and holes might be captured into different QDs,
resulting in QDs that are only populated either by electrons or by holes. In that situation the electron-hole scattering channel is blocked. However, even in case of p-shell excitation carriers can be scattered into the WL, for example by the processes depicted in Fig. 5.19a-b, and subsequently captured into a different QDs. This also results in QDs that are only populated either by electrons or by holes. Additionally, for later stages of the kinetics also WL assisted processes contribute, independent of the excitation condition. Furthermore, our procedure also includes conﬁgurations with QDs populated by more than one electron-hole pair even if the total carrier density is less than the QD density. An important point is that this is also the case in typical experimental situations. A weak pump pulse, that on average generates one electron-hole pair per QD, can in fact generate two electron-hole pairs in one QD and no electron-hole pair in another QD. This opens relaxation processes where for example two QD electrons or two QD holes are scattered. As an example the electron-electron scattering is depicted in Fig. 5.19a.
Our results show that for the low-temperature regime all scattering processes are important, even though electron-hole scattering dominates for early stages of the kinetics after optical pulse excitation. Due to polaron renormalizations, the carrier-LO-phonon interaction gives rise to scattering rates comparable to Coulomb scattering, even though the polaron spectral function exhibits narrow resonances at low temperatures.
(ii) Experimental analysis
The DTS signal shown in Fig. 5.18a contains additional contributions beyond the carrier-carrier and carrier-carrier-phonon scattering processes discussed above. Coulomb interaction of conﬁned carriers leads to so-called multi-exciton states [20, 140]. Also the carrier spin was not considered so far. Therefore a more detailed analysis is necessary to understand the experimental data.
A signiﬁcant contribution to the long-lived DTS signal might be due to so-called dark-exciton conﬁgurations rather than Pauli-blocking effects. Dark dark-excitons consist of an elec-tron and a hole, both having identical spin. For this conﬁguration optical transitions are forbidden and a carrier recombination requires a preceding spin-ﬂip process which is very unlikely on a ns timescale. Due to the optical selection rules, conventional pump-probe se-tups are only sensitive to bright-exciton transitions. Using linearly polarized probe pulses it can be detected for example if the QD s-shell is populated with one or two bright exci-tons. In contrast, a single dark exciton blocks both bright transitions. Thus, a level that is populated by two bright excitons cannot be distinguished from a dark exciton. As a consequence, in the DTS data shown in Fig. 5.18 the number of carriers detected in higher states might be overestimated.
To gain more insight into the population of the QD, additional measurements have been performed, where a magnetic ﬁeld is applied perpendicular to the incident pump and probe
beams (Voigt conﬁguration). In a classical interpretation, the carriers react to this perturba-tion with a precession of the carrier spins around the ﬁeld. The magnetic ﬁeld breaks the cylindrical symmetry of the system, and as a consequence the angular momentum is no longer a good quantum number. However, the resulting states can be described as a super-position of the unperturbed angular momentum states . As a consequence the bright-and dark-exciton states mix, resulting in an optical observability of all spin conﬁgurations.
This experimental setup allows a more adequate detection of the carrier populations as no optical transitions are blocked due to dark-exciton conﬁgurations.
The corresponding experimental results obtained in Voigt conﬁguration are presented in Fig. 5.21a. The dominating dark-exciton contribution to the ground state vanishes and an overall reduction of the DTS signal is observed. Also in Voigt conﬁguration long-lived traces are observed, especially for the excited states. As in this case no dark excitons contribute, Fig. 5.21a represents more accurately the QD population. Thus, the long-lived features for the excited states can be clearly assigned to resident carriers.
For additional information about the origin of the DTS traces an external magnetic ﬁeld in Faraday conﬁguration was applied, with the magnetic ﬁeld parallel to incident pump/probe beam in z-direction. The Zeeman splitting observed in the TRDT signal is depicted in Fig. 5.21b. Clearly an s-like, p-like and d-like splitting of the resonances is seen, conﬁrm-ing their interpretation as QD resonances.
The experimental results show fast carrier scattering for elevated temperatures and at low temperatures the emergence of a phonon bottleneck after fast initial relaxation. Within the quantum-kinetic description of carrier-scattering due to the interaction with LO phonons the experimental ﬁndings for both temperature regimes can be understood.
For elevated temperatures, the absence of a phonon-bottleneck is clearly veriﬁed by the fast rise time of the TRDT signal for the ground state, which does not depend on the ex-cited carrier density as shown in Fig. 5.18b. It has been discussed in detail in Chap. 5.2.1 that this is due to polaron effects. In case of low temperatures, Fig. 5.18b shows a much slower relaxation times and a clear dependence on the excitation density. Furthermore, an incomplete thermalization is observed in Fig. 5.21a, which is seen in the population of en-ergetically higher QD states for late times. Slow relaxation times can be understood by the much sharper resonances of the polaron spectral function in this temperature regime. Ad-ditionally, the quantum-kinetic calculation shows an incomplete thermalization of carriers in the long-time limit as depicted in Fig. 5.17.
Even though the experimental ﬁndings for both temperature regimes can be understood within our quantum-kinetic model for the carrier-LO-phonon interaction, in addition Cou-lomb effects might contribute in the experiment. For the particular experimental situation
(a) DTS spectrum (Voigt) (b) Zeeman splitting (Faraday)
Fig. 5.21: DTS spectrum on an ensemble of InGaAs QDs with an magnetic ﬁeld (7 T) ap-plied in Voigt conﬁguration (a) and Zeeman splitting of the QD traces in the DTS spectrum due to magnetic ﬁeld in Faraday conﬁguration (b). Pictures courtesy of H. Kurtze and Prof.
Dr. M. Bayer, University Dortmund.
it is difﬁcult to analyze the relative strength of carrier-carrier and carrier-LO-phonon scat-tering processes. Both mechanisms are competing, depending on the population conﬁgura-tion and temperature. As experimentally shown in Fig. 5.18b and theoretically conﬁrmed in Fig. 5.20, even in the low-carrier-density regime Coulomb scattering plays an important role in the relaxation of carriers towards the ground state. However, the non-thermal carrier distribution observed in the experiment is a signature of the interaction with LO-phonons.
For carrier-carrier scattering processes one expects a Fermi-Dirac distribution in the long-time limit, as any energy can be transferred to the scattering partner. Therefore, we can conclude that in Fig. 5.21a the kinetics is not dominated by Coulomb processes but by the interaction with LO phonons, even though both mechanisms contribute to the fast carrier relaxation.
In contrast to Chap. 5 where the focus is on carrier scattering, this chapter is dedicated to optical effects like coherent polarization dynamics and photoluminescence. Their impor-tance for the application of QDs in LED and laser devices has been already elaborated in Chap. 2. Semiconductor optics is a wide ﬁeld that ranges from wave-guide structures for light conﬁnement to quantum optics, light-matter coupling, and ultrafast carrier kinetics [18, 34]. In the following chapter we focus on the optical response and the photolumines-cence properties of semiconductor QDs.
To experimentally study the optical response of a semiconductor, nowadays well-established pump-probe experiments are available, using for example photon-echo or four-wave-mixing (FWM) conﬁgurations . For the discussion of the optical response basically two pic-tures are employed, depending on the excitation density regime. Whereas for high car-rier densities results are discussed by means of the many-body interaction of an electron-hole plasma, in the low-carrier-density regime the exciton picture is adequate, taking into account few-particle interactions. An example for a few-particle system are QDs in the low-temperature and low-excitation regime, where most of the carriers are in the ground state. This so-called multi-exciton regime is successfully described using the conﬁguration-interaction (CI) method in order to calculate the corresponding absorption spectra [20, 140, 157]. For high carrier densities, the coherent polarization dynamics can be described using the framework of NGFs, which follows similar lines as discussed for the carrier scattering in Chap. 5. Already early publications on the carrier kinetics included coherent polarization effects [57, 107]. Absorption spectra [158, 159] as well as ultra-fast phenomena in pump-probe experiments have been studied using this method [34, 58, 96].
An alternative approach is the dynamics-controlled truncation (DCT) developed by Axt and Stahl [69, 70], which was successfully used to study study exciton and biexciton reso-nances in FWM experiments and can also be formulated using NGFs [71, 73, 74]. Besides Coulomb effects like exciton and biexciton formation, mainly the dephasing due to the in-teraction with LA phonons has been investigated. For example the inﬂuence of dephasing on Rabi oscillations in QDs [160, 161], which are considered for application as optical switch. It has been pointed out that for the low-temperature regime LA phonons provide the dominant contribution, whereas at elevated temperatures also LO phonons play an im-portant role [44–46].
Our focus in Chap. 6.1 is on laser applications where elevated temperatures and high carrier-densities are present and hence the combined inﬂuence of Coulomb and phonon
effects is important. For the optical properties especially the inﬂuence of many-body renor-malizations like polaron effects, as well as the importance of different scattering channels is of interest.
The coherent optical response is governed by dephasing processes on a femto-second time scale. In contrast, photoluminescence experiments incorporating carrier recombination processes take place on a much longer timescale of nano seconds. For laser applications the carrier recombination dynamics is of central importance. The spontaneous and stimulated emission of photons provides the basic mechanism for laser operation, together with the optical feedback of the cavity. Interesting subjects of current research are for example single-photon sources , which can be used for quantum cryptography. These devices involve only a single QD as light emitter. Therefore, the light-matter interaction of the QD with the cavity mode is of special interest and is currently intensively investigated in the ﬁeld of the so-called cavity QED [18, 23, 26, 162]. Furthermore, single-photon sources show almost no threshold behavior in the input-output curve. However, the transition from spontaneous to stimulated emission can be seen in the photon statistics of the emitted light, which is investigated using corresponding correlation measurements [18, 163, 164].
For the theoretical description of such single-emitter devices, bridging the timescales for carrier scattering and recombination processes is one of the main problems. Optical coher-ences dephase rapidly but carrier scattering processes on a fs timescale strongly inﬂuence the recombination dynamics. They determine the population of the QD ground state as well as renormalizations of the single-particle states. The development of a model for the recombination dynamics and its incorporation in a laser model is a challenging task on its own. Detailed studies on this subject are presented for example in Refs. [67, 68, 165].
In this thesis, the focus of Chap. 6.2 is on bridging the different timescales and including carrier-scattering and quasi-particle renormalizations in the emitter model.